**Analysis of Thermal Conductivity of Frost on Cryogenic **

**Finned-tube Vaporizer Using Fractal Method **

**Shuping Chen, Shuting Yao, Fushou Xie **

School of Petrochemical Engineering, Lanzhou University of Technology, Lanzhou, China Email: [email protected]

Received March, 2013

**ABSTRACT **

Thermal conductivity of frost is not only related to density, but also affected by its microstructure and environmental conditions, and it will continuously change with the formation and growth of frost. Images of frost formation and growth on the cryogenic surface in various shapes at different stages were obtained by experimental measurements, and a numerical simulation of frost formation and growth was carried out based on Diffusion Limited Aggregation (DLA) model of fractal theory in this paper. Based on the frost structure obtained by experiment, the fractal dimensionof pore area distribution and porosity of frost layer on the cryogenic finned-tube vaporizer were calculated by using fractal me-thod, and combined with heat conduction model of frost layer obtained by thermal resistance meme-thod, the thermal con-ductivity of frost on the cryogenic surface was calculated. The result shows that the thermal concon-ductivity calculated by the fractal model coincides with the range of the experimental data. Additionally, comparison with other heat conduc-tion models indicated that it is feasible to introduce the fractal dimension of pore area distribuconduc-tion into heat conducconduc-tion model to deduce the thermal conductivity of frost.

**Keywords:** Cryogenic Finned-tube Vaporizer; Thermal Conductivity; Frost Layer; Fractal

**1. Introduction **

Finned-tube vaporizer will be frosted once its surface temperature is below the dew point of surrounding humid air, and lower than 0℃. The frost on the surface of va-porizer will decrease the efficiency of vava-porizer, increase the pressure loss and even result in the failure of the va-porizer system. Sublimation frosting of humid air on the vaporizer surface involves heat transfer, mass transfer and the boundary movement of special porous medium. Of all the issues concerning the sublimation frosting, frost physical properties especially the thermal conduc-tivity is one of the key parameters. There have been a lot of researches on the effect of thermal conductivity on frosting problem. At the beginning, researchers mainly concentrated on the experimental study of the formation and growth of frost on the simple geometric surfaces, such as level plate, pipe and vertical plate. Various em-pirical or semi-emem-pirical correlations of the density and thermal conductivity were proposed [1-7]. Then, numer-ous attempts on the growth and physical properties of frost on the cold plate or pipe based on the mechanism of frosting were made, too. Based on the mechanism of frosting, and considering the process of water vapor dif-fusion in frost, Brain [8] firstly put forward that water vapor flowing into the frost was divided into two parts, one part was used to increase the thickness of frost, the

other part to increase the density of frost. Hayashi Y [9] believed that the change of density essentially depended on the surface temperature of frost which was changing frequently in the process of frosting. According to the different structures at different growth and formation stages of frost, he demonstrated three periods which could describe the evolution of frost layer: the crystal growth period, the frost layer growth period, and the frost full-growth period, and finally proposed the well-known correlation for frost density in terms of frost temperature and ice-air mixture model. On the basis of the theory of Hayashi Y, considering the space distribution and time-varying of density and temperature of frost, Tao Y X [10] applied the control volume average method of porous medium into ice-air mixture model and improved the accuracy of the model. Le Call R [11] modified the boundary conditions and the permeability coefficient of water vapor in Tao Y X model, and focused on the effec-tive diffusion coefficient of water vapor, then, he got the distribution of density, temperature, thermal conductivity in frost. Chen H [12] further modified Tao Y X model, and set up a mathematic model of dynamic growth char-acteristics of frost on a flat plate.

used to describe the geometric distribution of frost. However, as a porous medium, the thermal conductivity of frost is not only related to density, but also affected by its microstructure and the environmental conditions. The thermal conductivity will continuously change with the formation and growth of frost, therefore, the thermal conductivity is a function of density, porosity, tortuosity and other parameters. The over-simplified frosting model will result in a serious error. The formation and growth of frost is a complicated process, therefore, it is very dif-ficult to obtain an equation of thermal conductivity based on a theory. Based on simulating the frost crystal struc-ture which has fractal growth characteristics, Cai L [13] set up an equilibrium equation at each node and predicted the thermal conductivity of frost by using the DLA mod-el. In the present paper, on the basis of the previous work, according to the experimental observation of frost forma-tion and growth, the physical process of frost growth was simulated by DLA (Diffusion Limited Aggregation) model of fractal theory. The box counting dimension method was used to determine the fractal dimension of pore area distribution and fractal porosity of frost profile. Thereby, a fractal model of heat conduction in frost layer was established theoretically to determine the effective thermal conductivity.

**2. Frost Formation and Growth Process **

The experimental facility utilized in this work is shown
in **Figure 1**. The facility is composed of the feeding

liq-uid system, the vertical frosting surface, the image
acqui-sition system and the data acquiacqui-sition system. This
ex-periment is conducted under the conditions of ambient
temperature *T*∞= 16.3℃, humidity *RH *= 55%, and these
environmental parameters remain unchanged during the
experiment. As shown in **Figure 1**, liquid nitrogen flows

from the liquid nitrogen tank, then through the vacuum thermal insulating tube to cryogenic vessel. The vacuum thermal insulating tube minimizes the loss of refrigera-tion capacity before liquid nitrogen flowing into the cryogenic vessel. Cryogenic vessel is welded by alumi-num flat plates, wrapped with the polyurethane foam material around it as the thermal insulation layer. A boss (with length of 120 mm, width of 100 mm, the height of 100 mm) is extended into the cryogenic vessel, and a vertical flat plate (with length of 120 mm, width of 100 mm) in the boss for frosting. Tubing is installed in the bottom of cryogenic vessel for connecting the cryogenic vessel and a glass level gauge, which is used to measure the height of the liquid nitrogen in the cryogenic vessel. Liquid nitrogen in cryogenic vessel absorbs heat by con-vection between the vertical flat plate and indoor humid air, and then gasifies; humid air will form frost on the surface of vertical flat plate.

**Figure 2** shows the experimental images of frost

growth on the cryogenic surface (with cryogenic surface
temperature *T*w= −120℃) at different time, it can be seen
from (a) and (b) that many dendritic frost crystals formed
on the cryogenic surface, and new dendritic crystals
produced with increasing time; as shown in (c), these
dendritic frost crystals are characterized with fractal
self-similarity to some extent [14, 15].

**Figure 3** shows the simulated image of frosting on the

cryogenic surface of finned-tube vaporizer in MATLAB based on the DLA model of fractal theory. The detailed algorithm of simulating frosting and simulation results have been reported previously [16].

**Figure 1. Experimental apparatus for frosting test.. **

**Figure 2. Experimental images of frosting on the cryogenic **
**surface. **

**3. Fractal Characteristics of Frost Layer **

**3.1. Fractal Dimension **

Taking irregular geometric shape as the research object, fractal geometry is put forward to describe irregular shape with self-similarity. The so-called fractal is the geometric object which has self-similarity in shape and structure, the mathematical expression of fractal is given by

*N*(*δ*)∝*δ*d_{ (1) }
Here, *N *is occupation space of a fractal object (the line,
the area or volume), *δ* is measurement scale, and *d* is
fractal dimension, it may be an integer or not an integer.
Fractal dimension is the measurement of the complexity
of fractal object, a quantitative parameter describing
fractal characteristics of an object. The larger value is,
the more complex the fractal object is. For a fractal area
with *d* between 1 and 2, its value can be determined by
the slope of curve in figure ln*N*(*δ*)-ln*δ* [17]. Fractal
structure is actually an ideal model and is an abstract of
many complex objects in nature. The true object in
na-ture is closer to random fractal, that is, random fractal
has self-similarity only in a certain scale range, called
statistical self-similarity. For example, the self-similarity
of porous medium is valid just in a certain scale.

Statistical self-similarity is usually called local fractal.
It has been proved that effective thermal physical
pa-rameter *E* of porous medium is not only related to the
medium’s property of its composition, but also depended
on the space structure of porous medium. According to
local fractal theory, if a porous medium has fractal
struc-ture and local fractal scale *l*, the effective thermal
physi-cal parameter of porous medium can be expressed as

( *i*, , ,

*E* *f*

###

*E*

*d l*) (2)

where *E*i is thermal physical parameter of each phase
composed of porous medium, *ε*is average volume
poros-ity of porous medium, *d* is fractal dimension. This
for-mula is the basic equation of determining thermal
physi-cal parameter of fractal object based on the fractal
the-ory.

Frosting is a transient process accompanied by air-
solid phase change, related with heat transfer, mass
transfer, and the boundary movement of porous medium.
Frost layer may be considered as a random porous
me-dium consisting of ice and air, just as shown in **Figure 2**.

Ice crystals skeleton of frost layer or pore is not uni-formly distributed on the profile surface, as it is hard to fill the entire profile of frost layer. In many cases, the area distribution of pore structure or ice crystals skeleton has fractal characteristics, therefore, the corresponding fractal dimension of area distribution for pore or ice crystals skeleton can be calculated. The specific

calcula-tion procedures are as follows:

1) As shown in **Figure 4**, taking any different

meas-urement values *X* in *D*～*A* interval.

2) Taking a point as the center of calculated area in
frost layer profile, the box with sides *X* is used for
meas-uring the area of pore in the calculated profile.

3) Repeat step (2) many times, until the whole frost
layer profile is measured with equal probability, and the
average value of pore area is *S*.

4) Change scale value *X*, and repeat the step (2) and
step (3), then a series of pore areas *S*i corresponding with
different scales *X*i can be obtained.

5) Using the least square method for linear fitting, the

*S*-*X* logarithm coordinates figure can be obtained.
It is clear that the average value *S* of pore area of frost
on the cryogenic surface and measurement scale *X *fit a
linearity in the *S*-*X* logarithm coordinates figure, and also
has the following linear relation:

Ln*S *= ln*k*+*d*ln*X* (3)
where *k *is a proportional constant, the slope *d* is the
fractal dimension of pore area distribution of frost layer.

**3.2. Fractal Porosity of Frost Layer **

For frost structure with certain porosity, as the pore area distribution of frost profile has fractal characteristics, the Equation (3) can be rearranged to:

*d*

*S* *k X* (4)
where *d* is fractal dimension of pore area distribution and

*S* is a measured average value.

By simplifying the actual irregular structure of frost
and assuming that the pore structure of frost as a cube,
where there is the cavity for air flowing through in the
middle of the cubical structure of frost, the rest of the
cubical structure is considered as frost ice crystals
skele-ton. Each calculation volume unit of frost layer is shown
in **Figure 5**. Since the similar structure has an invariant

property of scale, the heat transfer characteristics of every calculation volume unit of frost layer will keep in agreement with the whole frost crystal. Then the effec-tive volume porosity of frost based on the fractal theory is defined as:

**Figure 5. Model of volume unit of frost layer. **

2 3 2

### ( )

*S*

*X*

(5)

Substituting Equation (4) and Equation (5), then:

(1 )

*a* *ice*

(6) The density of frost based on the fractal porosity can be obtained by the reference [18]:

3
3 _{(} _{2)}

2

2 *d*

*k X*

_{}

(7)
where *ρ* is frost density, kg·m-3_{; }_{ρ}

a is air density, *ρ*a
=1.292 kg·m-3_{; }_{ρ}

ice is ice density, *ρ*ice =0.9×103 kg·m-3.

**3.3. Thermal Conductivity of Frost **

As a special porous medium, the actual microstructure of
frost is changeable and irregular. The local area fractal,
however, still exists from the above analyses. Therefore,
a simplified unit pore profile model of frost layer shown
in** Figure 6**. The simplified profile has the same pore

area and the same fractal dimension *d* of local pore area
with the original actual profile, and then they should
have the same effective thermal properties. For
simplify-ing the calculation, the simplified fractal model of heat
conduction in frost layer shown in **Figure 7** is adopted.

The thermal resistance *R* of the fractal model is shown
in **Figure 8 **and expressed as:

1 2

1 2

(

*i* *i* *a*

*i* *i* *a*

*R* *R* *R*

*R*

*R* *R* *R*

)
(8)
where
1
3
1 _{2}
3
1
(1 )
*i*
*i*
*R*

(9)

1 1
3 3
2 _{2}
3
(1 )
(1 )
*i*
*i*

*R*

(10)

2
3
1
*a*
*a*
*R*

(11)

1 2

3

2 _{2} _{2}

3 3

(1 ) (1 )

(1 )

*a* *i*

*i* *a*

*a* *i*

*R* *R*

Then 1 2 2 1 3 3 3

2 1 2 _{2} _{2} 2

3 3 3 _{3}

(1 )(1 ) (1 )

(1 ) (1 ) ( ) _{(1} _{)}

*i* *a*

*a*
*a* *i*

*R*

_{}
_{}

_{} (13)

The effective thermal conductivity of frost can be ex-pressed as:

2 1 2 _{2} _{2} 2

3 3 3 _{3}

1 2

2 1

3 3

3

(1 ) (1 ) ( ) _{(1} _{)}

1

(1 )(1 )
(1 )
*a*
*a* *i*
*i* *a*
*R*
_{}
_{}
_{}
_{}
(14)
where *λ*a is the thermal conductivity of air, *λ*a=0.024
W·m-1_{·}_{K}-1_{; }_{λ}

i is the thermal conductivity of ice, *λ*i=1.88
W·m-1_{·K}-1_{;λis the thermal conductivity of frost. }

**4. Results and Discussion **

**4.1. Discussion of Fractal Dimension **

The box counting dimension method is used to calculate
the fractal dimension *d* of pore area distribution of frost
for frosting simulation image shown in **Figure 3**, and

then being compared with the fractal dimension of
ex-perimental binary image shown in **Figure 9**. The

calcula-tion result is shown in** Figure 10**. The fractal dimension

**Figure 6. Schematic diagram of an unit pore profile. **

**Figure 7. Simplified heat conduction model of frost layer. **

3

[image:4.595.63.527.528.741.2]**Figure 9. Experimental frosting binary image on the **
**cryogenic surface of finned-tube vaporizer. **

**Figure 10. Linear fitting for the fractal dimension of pore **
**area distribution. **

of pore area distribution by simulation of frost is *d*1 =
1.743, and the fractal dimension of pore area distribution
from experimental frost is *d*2 = 1.466. It can be seen from

**Figure 10** that the profile pore distribution of frost on the

surface of finned-tube vaporizer satisfies statistical
self-similarity in measurement scale *D*~*A* interval,
namely, the pore distribution of frost profile presents
fractal characteristics. In addition, the consistent of the
fractal dimension of the simulation image *d*1 with that of
the experimental image *d*2 shows the rationality of the
numerical simulation and provides a powerful evidence
for further deriving the fractal model of heat conduction
in frost layer.

**4.2. Thermal Conductivity of Frost Layer **

It can be obtained that the diameter scale of pore space of
the actual frost layer is 1~20. In order to establish a
gen-eral fractal model of frost, a range of 1~20 is used as the
value of measurement scale *X* in** Figure 10**. As shown in
**Figure 10**, *d*1 = 1.743, *k*1 = 1.274, *d*2 = 1.466, *k*2 = 1.861,
substituting the related values into Equation (7), the
den-sity *ρ* of the actual frost can be calculated, as shown in

**Figure 11**. Then the thermal conductivity of actual frost

is got by Equation (14), shown in** Figure 12**. It can be

seen that the thermal conductivity of actual frost
calcu-lated by the above fractal model agrees well with the
range of0.02～0.16 W·m-1_{·K}-1 _{of the thermal }

conduc-tivity reported by reference, and thus explains the ration-ality of the fractal model of heat conduction.

**Figure 13** shows comparison between the proposed

model and other models. It has been generally accepted that the thermal conductivity of frost is considered to be depended on density. In fact, there are large differences

0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 100

200 300 400 500 600 700 800

Density ρ(k

g ·

m

-3 )

Porosity

**Figure 11. Density varied with the change of porosity. **

100 200 300 400 500 600 700 800

0.0945 0.0950 0.0955 0.0960 0.0965 0.0970

Therm

al conductivity λ(W·

m-1 ·K -1 )

[image:5.595.317.532.567.715.2]Density ρ (Kg· m-3 )

**Figure 12. Frost layer thermal conductivity varied with **
**the change of density. **

between each model shown in** Figure 13**. Therefore, it

shows that the thermal conductivity of frost is not only
depended on density, but also on the microstructure and
frosting environmental conditions. Curve No.1is obtained
from the maximum parallel model and Curve No.5 from
the minimum series model. These two curves represent
the limits of thermal conductivity of frost, and the curve
of thermal conductivity of actual frost should lie between
these two curves. Curve No.2 is the random mixture
model, which applies to the mixture of air and ice mixed
at certain proportion. But it has big deviation from
prac-tical case due to the soaring of thermal conductivity
un-der small porosity. The cubic lattice model Curve No.3
consists of open cubic lattice structure, with ice
deposit-ing on the edge of the lattice, where the moist air exists
between lattices. It can be seen from the **Figure 13** that

the thermal conductivity of this model is going up rapidly
in the low density, not in accordance with the real
situa-tion. Yonko-Sepsy model Curve No.4 considers frost as a
mixture of ice and air. The calculation result is more
practical, but this model is only valid to a certain range
of porosity [19]. Curve No.6 is obtained from the model
in the present paper. The modeling result lies in between
the minimum series model and Yonko-Sepsy model. The
model can be applied to the density of frost greater than
500 kg·m-3_{, that is, the frost turning into the scale of full }
growth and not restricted by the porosity. Therefore, the
thermal conductivity calculated by the above fractal
model coincides with the real situation better than other
models, and the thermal conductivity of frost has a wider
applicable scale.

**5. Conclusions **

The fractal dimension of pore area distribution and frac-tal porosityof frost profile were determined based on the observed structure of frost growth. Then, the heat con-duction model in frost layer is proposed by using fractal method, and the thermal conductivity is also expressed by a function of the fractal dimension of pore area dis-tribution and porosity of frost. The calculated result shows that thermal conductivity of frost obtained by the fractal model agrees well with the testing data of the ef-fective thermal conductivity. In addition, this fractal model of heat conduction is not restricted by the porosity, and will have broader application area compared to other models. It also verifies the feasibility of adopting the fractal dimension of pore area distribution into the model of heat conduction to determine thermal conductivity. The research shows that frost physical properties is of great importance in evaluating the heat transfer perform-ance of air-heating vaporizer under frosting conditions, which will help optimizing the structure of vaporizer and the defrosting time.

**6. Acknowledgements **

This study was supported by the National Natural Sci-ence Foundation of China No. 51076061.

**REFERENCES **

[1] H. W. Schneider, “Equation of the Growth Rate of Frost
Forming on Cooled Surface,” *International Journal of *
*Heat and Mass Transfer*, Vol. 21, No. 8, 1978, pp.
1019-1024. doi:10.1016/0017-9310(78)90098-4

[2] D. L. O 'Neal and D. R. Tree, “Measurement of Frost
Growth and Density in a Parallel Plate Geometry,”
*ASH-RAE Transactions*, Vol. 26, No. 5, 1984, p. 56.

[3] S. M. Sami and T. Duong, “Mass and Heat Transfer
dur-ing Frost Growth,” *ASHRAE Transactions*, Vol. 95, No. 1,
1989, pp. 158-165.

[4] D. K. Yang and K. S. Lee, “Dimensionless Correlations
of Frost Properties on a Cold Plate,” *International *
*Jour-nal of Refrigeration*, Vol. 27, No. 1, 2004, pp. 89-96.
doi:10.1016/S0140-7007(03)00118-X

[5] G. Biguria and L. A. Wenzel, “Measurement and Correla-tion of Water Frost Thermal Conductivity and Density,”

*Industrial and Engineering Chemistry Fundamentals*, Vol.
9, No. 1, 1970, pp. 129-138.doi:10.1021/i160033a021
[6] A. Z. ahin, “Effective Thermal Conductivity of Frost

During the Crystal Growth Period,” *International Journal *
*of Heat and Mass Transfer*, Vol. 43, No. 4, 2000, pp.
539-553. doi:10.1016/S0017-9310(99)00162-3

[7] C. H. Cheng and C. H. Shiu, “Frost Formation and Frost
Crystal Growth on a Cold Plate in Atmospheric Air
Flow,” *International Journal of Heat and Mass Transfer*,
Vol. 45, No. 21, 2002, pp. 4289-4303.

[8] P. L. T. Brian, R. C. Reid and Y. T. Shah, “Frost
Deposi-tion on Cold Surfaces,” *Industrial and Engineering *
*Chemistry Fundamentals*, Vol. 9, No. 3, 1970, pp.
375-380.

doi:10.1021/i160035a013

[9] Y. Hayashi, A. Aoki, S. Adachi and K. Hori, “Study of Frost Properties Correlating with Frost Formation Types,”

*Journal of Heat Transfer*, Vol. 99, No. 2, 1977, pp.
239-245.

doi:10.1115/1.3450675

[10] Y.-X. Tao, R. W. Besant and K. S. Rezkallah, “A
Mathe-matical Model for Predicting the Densification and
Growth of Frost on a Flat Plate,” *International Journal of *
*Heat and Mass Transfer*, Vol. 36, No. 2, 1993, pp.
353-363.

doi:10.1016/0017-9310(93)80011-I

[11] R. Le gall, J. M. Grillot and C. Jallut, “Modeling of Frost
Growth and Densification,” *International Journal of Heat *
*and Mass Transfer*, Vol. 40, No. 13, 1997, pp. 3177-3187.
doi:10.1016/S0017-9310(96)00359-6

[13] L. Cai, R. H. Wang, P. X. Hou and X. S. Zhang,
“Com-puter Simulation of Frost Growth and Computation of Its
Thermal Conductivity,” *Chinese Journal of Chemical *
*Engineering*, Vol. 60, No. 5, 2009, pp. 1111-1115.
[14] Y. L. Hao, I. Jose and X. T. Yong, “Experimental Study

of Initial State of Frost Formation on Flat Surface,”
*Jour-nal of Southeast University*, Vol. 35, No. 1, 2005, pp.
149-153.

[15] P. X. Hou, L. Cai and W. P. Yu, “Experimental Study and
Fractal Analysis of Ice Crystal Structure at Initial Period
of Frost Formation,” *Journal of Applied Sciences*, Vol. 25,
No. 2, 2007, pp.193-197.

[16] S. P. Chen, S. T. Yao, F. S. Xie, Z. X. Chang and H. Y.

Han, “Frost Model and Numerical Simulation of
Air-heating Fin-tube Vaporizer,” *Cryogenics & *
*Super-conductivity*, Vol. 39, No. 11, 2011, pp. 64-67.

[17] K. Falconer, “Fractal Geometry Mathematical Founda-tions and ApplicaFounda-tions,” W.Q. Zeng, TransacFounda-tions, Sec-ond edition, Posts &Telecom Press, Beijing, 2007, pp. 270-275.

[18] B. Na, “Analysis of Frost Formation in an Evaporator,” ph.D. Thesis, Pennsylvania State University, 2003. [19] J. D. Yonko and C. F. Sepsy, “An Investigation of the